- Nano Express
- Open Access
Effect of hydrogen treatment temperature on the properties of InGaN/GaN multiple quantum wells
Nanoscale Research Letters volume 12, Article number: 321 (2017)
InGaN/GaN multiple quantum wells (MQWs) were grown with hydrogen treatment at well/barrier upper interface under different temperatures. Hydrogen treatment temperature greatly affects the characteristics of MQWs. Hydrogen treatment conducted at 850 °C improves surface and interface qualities of MQWs, as well as significantly enhances room temperature photoluminescence (PL) intensity. In contrast, the sample with hydrogen treatment at 730 °C shows no improvement, as compared with the reference sample without hydrogen treatment. On the basis of temperature-dependent PL characteristics analysis, it is concluded that hydrogen treatment at 850 °C is more effective in reducing defect-related non-radiative recombination centers in MQWs region, yet has little impact on carrier localization. Hence, hydrogen treatment temperature is crucial to improving the quality of InGaN/GaN MQWs.
InGaN/GaN-based high-brightness light-emitting diodes (LEDs) have attracted tremendous attention over the past decade because of their applications in signage, back lighting, automotive headlights, and general illumination [1,2,3,4,5]. Despite of the great progress in materials and devices, there are still many unsolved issues related to the growth of InGaN/GaN multiple quantum wells (MQWs). One of the most serious problems is that the large lattice mismatch and low miscibility between InN and GaN result in the generation of several kinds of defects, such as alloy disordering, misfit dislocations, and stacking faults, which deteriorates the quality of MQWs [6, 7]. Generally, the typical growth temperature of InGaN quantum well (QW) for blue and green LEDs is below 800 °C to benefit indium incorporation [8, 9]. Meanwhile, the growth temperature of GaN quantum barrier (QB) is usually 50–150 °C higher than that of InGaN QW because of the low dissociation temperature of InN [6, 10]. Hence, the growth temperature of GaN barrier represents a compromise between the crystal quality of GaN and the In content in InGaN . The lower growth temperature of GaN QB can result in poor crystal quality of MQWs [12, 13]. Moreover, in order to alleviate indium desorption or re-evaporation during the temperature ramp-up and GaN QB growth process, a thin low-temperature GaN cap layer (LT-cap) is usually deposited immediately after the growth of InGaN QW layer [14,15,16,17]. Nevertheless, the crystal quality of GaN LT-cap layer is very poor. It is reported that increasing the thickness of LT-cap layer can seriously degrade the optical quality of InGaN/GaN MQWs [18, 19]. Hence, the quality of InGaN/GaN MQWs is inferior in general. Given the key role of MQWs in LEDs, obtaining high quality MQWs will bring huge gains in device performance. Up to now, many methods have been proposed, such as growth of GaN barriers using hydrogen as carrier gas [20, 21], growth interruption [22, 23], indium treatment [24, 25], staggered QWs [26,27,28], InGaN barrier [29,30,31], and Al(In)GaN cap layer [32,33,34]. Recently, Ren et al. reported that full H2 treatment on GaN barrier layer can enhance the optical quality of InGaN/GaN MQWs .
In this paper, a small H2 flow was introduced to treat the QW/QB upper interface before barrier layer growth, and the effect of treatment temperature on the optical and structural properties of InGaN/GaN MQWs was investigated. It was found that H2 treatment at 850 °C is more effective in reducing defect density, as demonstrated by the remarkably improved room temperature photoluminescence (PL) intensity, and the decreased surface roughness and pit density.
The InGaN/GaN blue emission MQW structures were grown on (0001) planar sapphire substrates by metal-organic chemical vapor deposition (MOCVD). The structure consisted of a 3.2-μm-thick nominally undoped GaN layer, and six pairs of InGaN/GaN MQWs with nominal 2.3-nm-thick InGaN wells separated by 10.5-nm-thick, lightly Si-doped (n-doping = 3 × 1017cm−3) GaN barriers. InGaN wells and GaN barriers were grown at 730 and 850 °C, respectively. A 1.0-nm-thick GaN LT-cap layer was deposited immediately after the growth of QW layer. Intervals without growth existed between each LT-cap and QB growth. Three samples with QW/QB upper interface treated at different conditions were prepared. Sample A, as the reference sample, employed pure N2 carrier gas during the temperature ramp-up process, while samples B and C were grown with 20 s H2 treatment, after each LT-cap layer growth but before the growth of each GaN barrier layer, at nominal treatment temperatures 730 and 850 °C, respectively. During the H2 treatment process, 200 sccm H2 was injected into the chamber.
High-resolution X-ray diffraction (HRXRD) measurement was performed using PANalytical Empyrean instrument to obtain the structure parameters. The PL properties were characterized by 325 nm He-Cd continuous wave laser, and the excitation power density was about 4.0 W/cm2. The temperature dependence of the luminescence spectra was measured from 10 to 300 K in a closed loop He cryostat. The luminescence was dispersed by a triple grating 50 cm monochromator and was detected by a GaAs photomultiplier tube using conventional lock-in technique. The surface morphology was studied by atomic force microscopy (AFM) (SPA-300HV) using tapping mode.
Results and discussion
Figure 1a shows HRXRD (0002) diffraction curves obtained by ω/2θ scans along the growth direction for the three samples. It can be seen that the simulation curves fit the experimental results very well. The satellite peaks up to the “−4th” order and Pendellösung fringes are clearly observed for the samples, indicating the fine periodic structure of MQWs, and the sharp interface between InGaN well and GaN barrier . The average indium content and well thickness of QW layer obtained by fitting the measured curves for samples A, B, and C are 10.95% and 2.30 nm, 10.76% and 2.32 nm, and 11.11% and 2.36 nm, respectively. The period thickness of MQWs for the three samples is kept around 13.80 nm. The full widths at half maximum (FWHMs) of InGaN “−1st” diffraction peak for the three samples are very close, as shown in Fig. 1b. The almost unchanged structural parameters indicate that the 1.0-nm-thick cap layer can effectively protect InGaN QW layer during the following H2 treatment process. The interface roughness can be calculated by fitting the FWHMs of the XRD satellite peaks using the following equation [18, 37]:
where ωn is the FWHM of the nth satellite peak, ω0 represents an intrinsic width of satellite peaks, Δθm is the angle spacing between the adjacent satellite peaks, and Λ0 is the period thickness of the InGaN/GaN MQWs. The slope of the fitting line is related to the interface roughness δ. The FWHM value as a function of satellite peak order is illustrated in Fig. 1b. It is obvious that sample C has a smaller absolute value of the slope, as compared with other two samples. Hydrogen treatment at 730 °C has little impact on interface roughness, as demonstrated by the little difference of slope value between samples A and B. These results indicate that interface modification is closely correlated with treatment temperature, and hydrogen treatment at higher temperature is beneficial to improving the interface quality.
The measured low temperature (10 K) and room temperature (300 K) PL spectra of the three samples are shown in Fig. 2. The observed multiple peaks come from Fabry-Perot interference fringes at substrate/GaN/air interface. The PL intensity at 10 K of the three samples changes a little. The PL peak energy (FWHM) at 10 K obtained by Gaussian fitting for samples A, B, and C is 2.711 eV (110 meV), 2.704 eV (100 meV), and 2.708 eV (99 meV), respectively. The nearly unchanged PL peak energy further reveals that 1.0-nm-thick GaN cap layer can effectively protect InGaN QW layer from indium loss during the H2 treatment process. The PL peak energy (FWHM) at 300 K obtained by Gaussian fitting for samples A, B, and C is 2.697 eV (158 meV), 2.696 eV (156 meV), and 2.698 eV (149 meV), respectively. It can be seen that the PL intensity at 300 K for sample A is close to that of sample B, while sample C shows a significant enhancement. The remarkable increase in room temperature PL intensity and decrease in line width for sample C indicate that H2 treatment at 850 °C is more effective in improving the optical qualities.
Figure 3 shows temperature-dependent integrated PL intensity of the three samples. It can be seen that the normalized integrated PL intensity shows monotonic decreasing behavior as the temperature increases, which can be well fitted using the following Arrhenius formula [38, 39]:
where I(T) represents the normalized integrated PL intensity. The parameters C 1 and C 2 are two constants related with the density of non-radiative recombination centers in the samples. E A1 and E A2 are the activation energies corresponding to the non-radiative recombination process. k B is Boltzmann’s constant. All the fitting results are listed in Table 1. It can be seen that the three samples have similar values of E A1 and E A2, meaning the unchanged types of non-radiative recombination centers after the interface treatment . The values of C 1 and C 2 for sample B are close to those of reference sample A, indicating that the number of non-radiative recombination centers is nearly unchanged when H2 treatment is conducted at QW growth temperature. In contrast, as the hydrogen treatment is carried out at QB growth temperature, the values of C 1 and C 2 significantly decrease from 2.35 to 1.40, and 112.77 to 62.77, respectively. The smaller C 1 and C 2 for sample C reveal that H2 treatment at high temperature can significantly reduce the density of non-radiative combination centers in MQWs region. As aforementioned, the crystal quality of GaN LT-cap layer is inferior as a result of the low growth temperature, which means the density of non-radiative recombination centers is high in this layer [18, 19]. Impurities, threading dislocations, V-pits and other defects are widely regarded as non-radiative recombination centers in InGaN/GaN MQWs, which are detrimental to the radiative recombination of carriers [41,42,43]. Piner et al. reported that adding a small amount of hydrogen into the carrier gas can significantly reduce carbon and oxygen concentrations in InGaN alloy, because hydrogen atoms can interact either with hydrocarbon radicals or with hydroxyl radicals to form highly stable products (CH4, H2O) . Hydrogen molecules thermally dissociate to hydrogen atoms at high temperature and the dissociation rate increases exponentially as the temperature rises . Besides, the high temperature promotes the volatile products desorption and outdiffusion from GaN surface. Therefore, more carbon and oxygen impurities at LT-GaN surface can be removed at high temperature. Furthermore, impurities and indium atoms can easily segregate to and diffuse along the dislocations, V-pits, and stacking faults, because of the presence of dangling bonds or local stresses or electrical fields in these areas [46, 47]. It is reported that threading dislocations propagating through GaN buffer layer lead to the formation of V-pits in MQWs region, while using higher growth temperature or hydrogen as the carrier gas can reduce the density and size of V-pits [23, 48]. Recently, Yeh at al. reported that hydrogen treatment at high temperature can etch away threading dislocations (TDs) in GaN templates . However, it is difficult to etch away TDs under low temperature (730 ~ 850 °C) and small hydrogen flow (200 sccm). The etching effect on the LT-GaN surface is very weak, as evidenced by the almost unchanged structural parameters of the MQWs. Nevertheless, hydrogen can react with indium atoms segregated at TDs to form volatile indium-hydride species, which desorbed rapidly at high temperature . Hydrogen can also diffuse along the dislocation line and react with impurities during the treatment duration. Because the treatment temperature for sample C is 120 °C higher than that of sample B, more hydrogen atoms are available from H2 pyrolysis. Moreover, the reaction rates between hydrogen atoms and defects (impurities and indium atoms segregated at TDs) would increase fastly as the temperature rises. As a result, the abovementioned defects can be reduced more efficiently after the hydrogen treatment conducted at higher temperature, which consequently contributes to the remarkable improvement in optical qualities for sample C.
In order to elucidate the physical origin of the improvement in optical qualities, temperature-dependent peak energy of the three samples is shown in Fig. 4. All the samples exhibit S-shaped curves, which is a typical feature of the localization effect in InGaN/GaN MQWs structures . The redistribution of carriers in the deep and shallow localized centers contributes to the first red-shift and then blue-shift of peak energy, as the temperature increases from 10 to 150 K. With further increase in the temperature to 300 K, the temperature induced band-gap shrinkage contributes to the red-shift of peak energy . The localization energy (σ) can be obtained by fitting the temperature-dependent peak energy curve using Band-tail model [53, 54]. The obtained localization energy for samples A, B, and C is 12.57, 12.34, and 13.30 meV, respectively, as shown in Table 1. The very small change in the localization energy indicates the negligible impact of hydrogen treatment on the depth of carrier localization. This result is quite different from the work by Ren et al., in which the degree of carrier localization would be enhanced after hydrogen treatment . In their work, hydrogen treatment was presented at the barrier surface by 1000 sccm H2, while other gases and precursors were switched off during the treatment. The difference may arise from that the hydrogen treatment here is conducted after the deposition of LT-cap layer and only 200 sccm H2 is added to the carrier gas to treat QW/QB upper interface. Under these conditions, the surface fluctuation caused by hydrogen treatment would be negligible. In other words, the undulating surface, favorable for the formation of phase segregation and quantum dot, is not satisfied [55, 56]. Consequently, the localization energy is almost unchanged after hydrogen treatment. Most importantly, these results verify that the enhancement of optical quality originates from the decreased density of defects in active region, rather than carrier localization.
The surface morphology of the samples tested by AFM is shown in Fig. 5. Atomic steps and pits are clearly observed in all samples. The calculated root mean square (RMS) surface roughness and pit density of the three samples are 0.619 nm and 1.96 × 108 cm−2, 0.601 nm and 2.00 × 108 cm−2, and 0.496 nm and 1.48 × 108 cm−2, respectively. It is obvious that introducing hydrogen treatment at 850 °C is beneficial in reducing surface roughness and pit density, while hydrogen treatment at 730 °C has little impact on surface quality. The difference in surface qualities between samples B and C may originate from the more effective removal of impurities, indium atoms segregated at TDs, and pits in active regions by H2 under higher temperature, as aforementioned. As a result, the decreased defect density can enhance the two-dimensional growth of barrier layer and beneficial in forming flat surface and sharp interface between well and barrier layer [57, 58]. Consequently, both the surface and interface qualities are improved by employing hydrogen treatment at 850 °C.
In summary, the effects of hydrogen treatment at different temperatures on optical and structural characteristics of InGaN/GaN MQWs are investigated. It is found that the degree of carrier localization is independent on hydrogen treatment, while hydrogen treatment at 850 °C can effectively reduce the non-radiative recombination centers in MQWs region. However, the sample with hydrogen treatment at 730 °C shows similar properties with the reference one. Hence, treatment temperature is an important parameter to improve the crystal quality of MQWs during hydrogen treatment process. Moreover, the physical origin of huge enhancement of room temperature PL intensity for the sample treated at 850 °C is the decreased defect density in MQWs accompanied by improved interface and surface qualities, rather than carrier localization.
Atomic force microscopy
Full width at half maximum
High resolution X-ray diffraction
Metal-organic chemical vapor deposition
Multiple quantum well
Cho J, Schubert EF, Kim JK (2013) Efficiency droop in light-emitting diodes: challenges and countermeasures. Laser Photonics Rev 7(3):408–421
Jia H, Guo L, Wang W, Chen H (2009) Recent progress in GaN-based light-emitting diodes. Adv Mater 21:4641–4646
Zhao H, Liu G, Zhang J, Arif RA, Tansu N (2013) Analysis of internal quantum efficiency and current injection efficiency in III-nitride light-emitting diodes. J Disp Technol 9(4):212–225
Lu T, Li S, Liu C, Zhang K, Xu Y, Tong J et al (2012) Advantages of GaN based light-emitting diodes with a p-InGaN hole reservoir layer. Appl Phys Lett 100(14):141106
Zhang YY, Yin YA (2011) Performance enhancement of blue light-emitting diodes with a special designed AlGaN/GaN superlattice electron-blocking layer. Appl Phys Lett 99:221103
Du C, Ma Z, Zhou J, Lu T, Jiang Y, Zuo P et al (2014) Enhancing the quantum efficiency of InGaN yellow-green light-emitting diodes by growth interruption. Appl Phys Lett 105:071108
Fischer AM, Wei YO, Ponce FA, Moseley M, Gunning B, Doolittle WA (2013) Highly luminescent, high-indium-content InGaN film with uniform composition and full misfit-strain relaxation. Appl Phys Lett 103:131101
Zhang Z-H, Tan ST, Ji Y, Liu W, Ju Z, Kyaw Z et al (2013) A PN-type quantum barrier for InGaN/GaN light emitting diodes. Opt Express 21(13):15676
Yang GF, Chen P, Yu ZG, Liu B, Xie ZL, Xiu XQ et al (2012) Temperature dependent growth of InGaN/GaN single quantum well. Superlattice Microst 52:349–356
Lv W, Wang L, Wang J, Hao Z, Luo Y (2012) InGaN/GaN multilayer quantum dots yellow-green light-emitting diode with optimized GaN barriers. Nanoscale Res Lett 7:617
Olaizola SM, Pendlebury ST, O’Neill JP, Mowbray DJ, Cullis AG, Skolnick MS et al (2002) Influence of GaN barrier growth temperature on the photoluminescence of InGaN/GaN heterostructures. J Phys D Appl Phys 35:599–603
Kim S, Lee K, Park K, Kim C-S (2003) Effects of barrier growth temperature on the properties of InGaN/GaN multi-quantum wells. J Cryst Growth 247:62–68
Kumar MS, Park JY, Lee YS, Chung SJ, Hong C-H, Suh E-K (2007) Effect of barrier growth temperature on morphological evolution of green InGaN/GaN multi-quantum well heterostructures. J Phys D Appl Phys 40:5050–5054
Hu Y-L, Farrell RM, Neufeld CJ, Iza M, Cruz SC, Pfaff N et al (2012) Effect of quantum well cap layer thickness on the microstructure and performance of InGaN/GaN solar cells. Appl Phys Lett 100:161101
Ju J-W, Kim H-S, Jang L-W, Baek JH, Shin D-C, Lee I-H (2007) A well protection layer as a novel pathway to increase indium composition: a route towards green emission from a blue InGaN/GaN multiple quantum well. Nanotechnology 18:295402
Pendlebury ST, Parbrook PJ, Mowbray DJ, Wood DA, Lee KB (2007) InGaN/GaN quantum wells with low growth temperature GaN cap layers. J Cryst Growth 307:363–366
Tao YB, Chen ZZ, Yu TJ, Yin Y, Kang XN, Yang ZJ et al (2011) Improvement of structural and luminescence properties in InGaN/GaN multiple quantum wells by symmetrical thin low temperature-GaN layers. J Cryst Growth 318:509–512
Yang J, Zhao DG, Jiang DS, Chen P, Zhu JJ, Liu ZS et al (2015) Optical and structural characteristics of high indium content InGaN/GaN multi-quantum wells with varying GaN cap layer thickness. J Appl Phys 117:055709
Li Z, Liu J, Feng M, Zhou K, Zhang S, Wang H et al (2013) Suppression of thermal degradation of InGaN/GaN quantum wells in green laser diode structures during the epitaxial growth. Appl Phys Lett 103:152109
Suihkonen S, Lang T, Svensk O, Sormunen J, Törmä PT, Sopanen M et al (2007) Control of the morphology of InGaN/GaN quantum wells grown by metalorganic chemical vapor deposition. J Cryst Growth 300:324–329
Czernecki R, Grzanka E, Smalc-Koziorowska J, Grzanka S, Schiavon D, Targowski G et al (2015) Effect of hydrogen during growth of quantum barriers on the properties of InGaN quantum wells. J Cryst Growth 414:38–41
Moon Y-T, Kim D-J, Song K-M, Choi C-J, Han S-H, Seong T-Y et al (2001) Effects of thermal and hydrogen treatment on indium segregation in InGaN/GaN multiple quantum wells. J Appl Phys 89(11):6514–6518
Ting SM, Ramer JC, Florescu DI, Merai VN, Albert BE, Parekh A et al (2003) Morphological evolution of InGaN/GaN quantum-well heterostructures grown by metalorganic chemical vapor deposition. J Appl Phys 94(3):1461–1467
Feng S-W, Lin H-C, Chyi J-I, Tsai C-Y, Huang CJ, Wang H-C et al (2011) The impact of trimethylindium treatment time during growth interruption on the carrier dynamics of InGaN/GaN multiple quantum wells. Thin Solid Films 519:6092–6096
Lee Y-J, Chen Y-C, Lu T-C (2011) Improvement of quantum efficiency in green light-emitting diodes with pre-TMIn flow treatment. J Phys D Appl Phys 44:224015
Arif RA, Ee Y-K, Tansu N (2007) Polarization engineering via staggered InGaN quantum wells for radiative efficiency enhancement of light emitting diodes. Appl Phys Lett 91:091110
Zhao H, Liu G, Li X-H, Huang GS, Poplawsky JD, Penn ST et al (2009) Growths of staggered InGaN quantum wells light-emitting diodes emitting at 520-525 nm employing graded growth-temperature profile. Appl Phys Lett 95:061104
Zhao H, Liu G, Zhang J, Poplawsky JD, Dierolf V, Tansu N (2011) Approaches for high internal quantum efficiency green InGaN light-emitting diodes with large overlap quantum wells. Opt Express 19(S4):A991–A1007
Lee W, Kim M-H, Zhu D, Noemaun AN, Kim JK, Schubert EF (2010) Growth and characteristics of GaInN/GaInN multiple quantum well light-emitting diodes. J Appl Phys 107:063102
Lin Z, Wang H, Lin Y, Yang M, Wang W, Li G (2016) Influence of In content in InGaN barriers on crystalline quality and carrier transport of GaN-based light-emitting diodes. J Phys D Appl Phys 49:115112
Zhang F, Ikeda M, Zhang S-M, Liu J-P, Tian A-Q, Wen P-Y et al (2016) Reduction of polarization field strength in fully strained c-Plane InGaN/(In)GaN multiple quantum wells grown by MOCVD. Nanoscale Res Lett 11:519
Koleske DD, Fischer AJ, Bryant BN, Kotula PG, Wierer JJ (2015) On the increased efficiency in InGaN-based multiple quantum wells emitting at 530-590 nm with AlGaN interlayers. J Cryst Growth 415:57–64
Hwang J-I, Hashimoto R, Saito S, Nunoue S (2014) Development of InGaN-based red LED grown on (0001) polar surface. Appl Phys Express 7:071003
Liu G, Zhang J, Tan C-K, Tansu N (2013) Efficiency-droop suppression by using large-bandgap AlGaInN thin barrier layers in InGaN quantum-well light-emitting diodes. IEEE Photonics J 5(2):2201011
Ren P, Zhang N, Xue B, Liu Z, Wang J, Li J (2016) A novel usage of hydrogen treatment to improve the indium incorporation and internal quantum efficiency of green InGaN/GaN multiple quantum wells simultaneously. J Phys D Appl Phys 49:175101
Wang W, Yang H, Li G (2013) Growth and characterization of GaN-based LED wafers on La0.3Sr1.7AlTaO6 substrates. J Mater Chem C 1:4070–4077
Tsai M-T, Chu C-M, Huang C-H, Wu Y-H, Chiu C-H, Li Z-Y (2014) The effect of free-standing GaN substrate on carrier localization in ultraviolet InGaN light-emitting diodes. Nanoscale Res Lett 9:675
Fang Y, Wang L, Sun Q, Lu T, Deng Z, Ma Z et al (2015) Investigation of temperature-dependent photoluminescence in multi-quantum wells. Sci Rep 5:12718
Soh CB, Liu W, Yong AM, Chua SJ, Chow SY, Tripathy S et al (2010) Phosphor-free apple-white LEDs with embedded indium-rich nanostructures grown on strain relaxed nano-epitaxy GaN. Nanoscale Res Lett 5:1788–1794
Wang Y, Pei XJ, Xing ZG, Guo LW, Jia HQ, Chen H et al (2007) Effects of barrier growth temperature ramp-up time on the photoluminescence of InGaN/GaN quantum wells. J Appl Phys 101:033509
Le LC, Zhao DG, Jiang DS, Li L, Wu LL, Chen P et al (2012) Carriers capturing of V-defect and its effect on leakage current and electroluminescence in InGaN-based light-emitting diodes. Appl Phys Lett 101:252110
Yang J, Zhao DG, Jiang DS, Chen P, Liu ZS, Zhu JJ et al (2016) Emission efficiency enhanced by reducing the concentration of residual carbon impurities in InGaN/GaN multiple quantum well light emitting diodes. Opt Express 24(13):13824
Yang Y, Cao XA, Yan CH et al (2009) Rapid efficiency roll-off in high-quality green light-emitting diodes on freestanding GaN substrates. Appl Phys Lett 94:041117
Piner EL, Behbehani MK, EI-Masry NA, Roberts JC, McIntosh FG, Bedair SM (1997) Impurity dependence on hydrogen and ammonia flow rates in InGaN bulk films. Appl Phys Lett 71(14):2023–2025
Chen JT, Forsberg U, Janzén E (2013) Impact of residual carbon on two-dimensional electron gas properties in AlxGa1-xN/GaN heterostructure. Appl Phys Lett 102:193506
Duxbury N, Bangert U, Dawson P, Thrush EJ, Van der Stricht W, Jacobs K et al (2000) Indium segregation in InGaN quantum-well structures. Appl Phys Lett 76:1600–1602
Pizzini S (1999) Chemistry and physics of segregation of impurities at extended defects in silicon. Phys Status Solidi (a) 171:123–132
Florescu DI, Ting SM, Ramer JC, Lee DS, Merai VN, Parkeh A et al (2003) Investigation of V-Defects and embedded inclusions in InGaN/GaN multiple quantum wells grown by metalorganic chemical vapor deposition on (0001) sapphire. Appl Phys Lett 83(1):33–35
Yeh Y-H, Chen K-M, Wu Y-H, Hsu Y-C, Yu T-Y, Lee W-I (2011) Hydrogen etching of GaN and its application to produce free-standing GaN thick films. J Cryst Growth 333:16–19
Koleske DD, Wierer JJ Jr, Fischer AJ, Lee SR (2014) Controlling indium incorporation in InGaN barriers with dilute hydrogen flows. J Cryst Growth 390:38–45
Li X, Zhao DG, Yang J, Jiang DS, Liu ZS, Chen P et al (2016) Influence of InGaN growth rate on the localization states and optical properties of InGaN/GaN multipl e quantum wells. Superlattice Microst 97:186–192
Lu T, Ma Z, Du C, Fang Y, Wu H, Jiang Y et al (2014) Temperature-dependent photoluminescence in light-emitting diodes. Sci Rep 4:6131
Eliseev PG, Perlin P, Lee J, Osiński M (1997) “Blue” temperature-induced shift and band-tail emission in InGaN-based light sources. Appl Phys Lett 71(5):569–71
Weng G-E, Zhao W-R, Chen S-Q, Akiyama H, Li Z-C, Liu J-P et al (2015) Strong localization effect and carrier relaxation dynamics in self-assembled InGaN quantum dots emitting in the green. Nanoscale Res Lett 10:31
Park I-K, Kwon M-K, Baek S-H, Ok Y-W, Seong T-Y, Park S-J et al (2005) Enhancement of phase separation in the InGaN layer for self-assembled In-rich quantum dots. Appl Phys Lett 87:061906
Park I-K, Park S-J (2011) Green gap spectral range light-emitting diodes with self-assembled InGaN quantum dots formed by enhanced phase separation. Appl Phys Express 4:042102
Fang ZL, Lin DQ, Kang JY, Kong JF, Shen WZ (2009) Interface modification of the InGaN/GaN quantum wells: the strain pre-relief effect. Nanotechnology 20:235401
Bruckbauer J, Edwards PR, Sahonta S-L, Massabuau FC-P, Kappers MJ, Humphreys CJ (2014) Cathodoluminescence hyperspectral imaging of trench-like defects in InGaN/GaN quantum well structures. J Phys D Appl Phys 47:135107
This work was supported by National Natural Science Foundation of China (Grant Nos. 61504090, 21471111, and 61604104), the Applied Basic Research Projects of Shanxi Province (Grant No. 2016021028), the National Key R&D Program of China (2016YFB0401803), and the Shanxi Provincial Key Innovative Research Team in Science and Technology (Grant No. 201605D131045-10).
YZ and TL conceived the study. YZ, XZ, and GZ conducted the sample growth and test experiments. YZ, TL, HD, ZJ, XL, and BX analyzed the data. TL and BX supervised the entire research project. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Zhu, Y., Lu, T., Zhou, X. et al. Effect of hydrogen treatment temperature on the properties of InGaN/GaN multiple quantum wells. Nanoscale Res Lett 12, 321 (2017). https://doi.org/10.1186/s11671-017-2109-6
- Treatment temperature
- Multiple quantum wells